Evolution of Asphalt Mixes – Innovations in FranceHigh modulus mixes – New wearing coursesRecycling – Warm AsphaltYves BrosseaudLaboratoire Central des Ponts et Chaussées – Francewww.ifsttar.frYves.firstname.lastname@example.org
Framework Evolutions bituminous mixes on wearing courses Evolutions of structural bituminous mixes Mains innovations• Very thin asphalt mixes BBTM or VTAC• Noise reduction wearing course, specific BBTM• Porous asphalt• Warm asphalt mixes• Colours in asphalt, high resistance to rut, to skid, … Conclusion
Evolution of the need for wearing courses 1960: Structural strengthening : Thick AC (6to10cm) [BBSG] 1975: Surface maintenance : Thin AC (4to5cm) [BBM]on good quality of underneath layers (structural and evenness) 1985 – 2000 : Specific surface maintenance :• Skid resistance : Very thin AC (2to3cm) [BBTM], Ultrathin AC (1cm)[BBUM]• Comfort, Visibility : Porous AC (4 cm) [BBDr]• Aesthetic with fine maximum size : Very thin AC (0/6 gap) [BBTM 0/6]• Decreasing of tire noise : BBTM 0/6, or BBDr in very thin layer• Heavy rutting resistance : Special AC• Decreasing of fatigue damage : High modulus AC [BBME]
Trends in bituminous mixtures evolutionsDissociation of layer functions :wearing course = surface caracteristics.base = structure
Wearing courses: main evolutions Thinner and thinner thickness1 to 2cm Reduction of maximum size : 14 / 10 / 8 / 6 / 4 mm Mix designGap graded formula Mix with more and more gravels Higher and higher porosityTack coat with seal properties More frequent use of polymer modified binder or specialbinder Hot mixes; except for microsurfacing [ECF] Standardized productsPerformance requirements
Definitions of asphalt wearing coursesSurface layerInternational nameBBSG (Béton Bitumineux Semi Grenus)BBME (Béton bitumineux à module élevé)DAC (Dense Asphalt)DAC with high performanceThickness,(cm)5-8BBM (Béton Bitumineux Minces) TAC (Thin Layer Surfacing) 3-4BBDr (Béton Bitumineux drainant) PA (Porous Asphalt) 4BBTM (Béton Bitumineux Très Mince) VTAC (Very Thin Layer) 2-3BBUM (Béton Bitumineux Ultra Mince) UTAC (Ultra Thin Layer) 1Good compromise between High skidding resistanceand Low noise pavements
Ranking of wearing coursescm9876540/10 sometime 0/14ThickBBSGBBMEThinTSBBM0/10 or 0/6 well gap gradedBinder BmPPABBDrThicknessMaximum size D, GradingFunction,Surface Characteristics321Very --- Ultra ThinBBTM VTACUTACBBUM
Main characteristics of ACType BB BBSG BBM BBTM BBUM BBDr ECFD 10 - 14 10 6 - 10 6 - 10 (6) - 10 6-8- 10Grading Cont. Gap. Gap. Gap. Gap. C. or G.% GSC 4 to 9 6 to 12 6 to 25 - 20 to 28 -Thick (cm) 6 to 8 3 to 5 2 to 2.5 1 to 1.5 3 to 4 1Spread (kg/m²) 150 to 200 100 40 to 60 25 to 35 80 15 à 20Tack coat (kg/m²)250 300 300 + 400 300 withoutSurface/year 5 6 27 1,5 1,5 30(million m²)Years of use 25 20 15 10 15 15Network All RN-RD All (A) RD A RD-townMarch 2005 – assessment : only the order of magnitude
Cut of Asphalt ConcreteReference : Thick ACGap graded VTACPorous AC
Base materials evolution Higher and higher binder contents Smaller aggregate maximum size :• 31 20 14 10 mm Increase of bitumen hardness:• 50 35 20 10 pen Additives to increase hardness Performances improvement• GB 3 then GB 4• EME 2 Reduction of thicknesses
Base and foundation materials evolution140120100806040% bitumeGradeModule2001970 1980 1990 2000 EME
Dissociation of road functions(since more than 15 years) Base course : structural effect• sufficient modulus to reduce the force on soil,• good fatigue resistance,• excellent stability in term of rutting resistanceHMA Wearing course : all surface characteristics• skidding resistance,• water proofing,• roughness,• visibility,• noise• recycling possibilityVTAM
Long term skid resistancecumulative traffic between 1 to 5 millions of trucksMaximum size of mixes D = 10 mmVTACUTACTACThick AC
Noise data : + 300 filesWearing courses : noise levelsLOW noiseIntermediatesNOISY78dBa75dBa7, 50 mRevêtement àtester1, 20 mExtract from data base of LRPC Strasbourg 2003
Low noise pavementBefore arriving here …. «Phonic» asphalt mixesUse low noise pavement• Low max size : 6 – 8 mm• Gap graded: 2/4• Polymer binder• Additives (sometimes)• Thickness : thin or very thin• Porous• High texture (SPT > 1 mm)• Good homogeneity• Excellent unevenness
联 通 、 非 联 通 和 封 闭 空 隙 Porous asphalt Operational since 1985 : motorway, ring roads, specific areas > 20% voids content (communicated) Less used today : winter maintenance, durability ofefficiency voids (clogging) Porous structure
Use of Polymers modified bitumen PmBTest on binders Ageing Complex Modulus Resistance to tensile (SHRP) Elastic recovery (elastomeric) Relaxation capacity with BBR (SHRP) Cohesion with pendulum (binder for surface dressing) Spectrometry, Chromatography, Distillation simulated (Expertise)- Test on asphalt concrete Mix design program Shear resistance (constrain under traffic)< 3% 3 to 5 % > 5%Microstructure of PmB SBS vs % polymer
Assessment to use PmBHow can it possible to improve the shear resistance with the binder of AC ?
Device to assess the resistance to shear stressesPatent Number FR 06 50 054 January 06, 2006Article BLPC, N° 267, avril 2007 - http://www.lcpc.fr/fr/sources/blpcliant modifié
Evolution of surface under testWay of load application
Resistance to shear stresses14Mass loss per unit of loaded surface area (kg/m2121086420Pull-out test performed on a BBTM 0/10 at room temperatureBinder ABinder CBinder BBinder DBinder EBmP0 2000 4000 6000 8000 10000 12000 14000 16000 18000 20000[Hamlat,2007]Number of loading cyclesliant modifié
0 20 40 60 80 100 120 140 160 180°C Kg/TTerminologyWAMLatent heat vaporization of water :537 kcal/kgHotmixasphaltHEATINGVAPORIzATION7654ColdasphaltSemi-warmasphaltÉnergie de chauffage (Kg/T)WarmasphaltDRYING3210
What’s look for WAM?Advantages:Reduction of energy consumptionLess pollution, concerning‣ People (workers, users, bordering the road)‣ Environment conditions Decreasing of bitumen ageing during production Less wear on mixing plant WITH the same performances as hot mixesContinue coating, final properties just after placement
No visible fumesNO visible steamsExempleWAM avec additifsagent plastifiantQuelques PhotosNO urgency, have timeGood homogeneityCleanWarmTemperatureGood workabilityUniformityWell aspect of joint
Main conclusion of WMAWarm modulus asphalt mix• Reduction of temperature : - 30 to 70°C• Main types of WAM processes used inFrance• Additives• Special binder1200000• Special heating1000000• Even with very high viscosity binder800000600000• Performances (laboratory – in 400000 field)• Same order of magnitude regarding:200000− Workability*0− Rutting resistance− Modulus and fatigue resistance− Densityestimation des tonnages BB Tièdes en France2004 2005 2006 2007 2008 2009 2010
Techniques for recycling of reclaimed asphaltPollutants?Classification from Direct-mat:european research project on recycling material in the road
Hot recycling asphalt on mixing plantRecycling in place in hotor cold conditions
Some figures : RAP in USA –Japan - EuropeM tons - %500450400350300250200150100500HMA - RAP in World : USA - Japan - Europe in2009?RAP in MtUSA Europe JapanAnnual production Mt% Recycling RAP in HMA% reused in road?
Some figures : various situationsin recycling160140120RAP in HMA - 2009RAP available 100000t% hot recycling% RAP HMA/total HMA100000 t or %100806040200NertherlandGermanySwedenSpainDenmarkBelgiumSwitzerlandFranceItaly
Use of Reclaimed Asphalt [%]100%90%80%70%60%50%40%30%20%10%0%Use of reclaimed asphalt material in road (2008)NetherlandsPercentage of differentend-of-life strategiesfor reclaimed asphaltGermanySwedenRomaniaDenmarkBelgiumSloveniaGenerally all RAP is used in or near roadOtherRecycling in unbound layersIn Situ / Plant Recycling (half warm & cold)Plant Recycling in HMASwitzerlandSpainHungaryzech RepublicFranceIrelandScource: EAPA 2008NorwayAustriaPoland
Some modifications due tosustainable developmentEvolution of recycling RAP in HMA in FRANCEMtons or %706050403020100RAP available Mt% RAP in HMA% RAP in HMA/HMA2001 2003 2005 2007 2008 2009Voluntary agreement for SD signed in 2009 by private road companies and Frenchadministration : Objective 2012 :RAP used in HMA 60% 2020road)2020 reused 100% soil @ road materials (back
Limits due to plant equipmentsExample : batch plantWithout specific deviceRate of reclaim ≤ 15%With ring for recyclingRate of reclaim ≤ 35%Double drumsRate of reclaim ≥ 50%Double barrel
Preliminary study in lab is essential Assess the sources : homogeneity RA Identification of components (on different sections and layers):binder content and residual properties, granularity of milling, EN 13108-8 Standards(others) Formula of new mix with RA (rate of recycling, nature ofbitumen or rejuvenator added, and aggregates) Performances must be equal to those of new AC Promote used of RAP : example in France no new study ifthe rate of recycling is less than:< 10% in wearing course< 15 % in binder, base, sub base courses (researches, publications LCPC/USIRF) Traditional pavement design study
Processes of recycling In practice:• What limits? What rate of recycling?• Binder : Penetrabilities, RBT, % asphaltènes?• Technology and environmental limits :• No sufficient homogeneity of mix,• Consumption energy• Fumes and streams emitted (toxicity)• Equipments of mixing plant• … Rejuvenator binder:• large scale available, but low market and lowdevelopment today, in the future?
Assessment after 30 years ofexperience in RAP Rate RAP in new HMA various : 10 to 70%• Current average near 20 to 25% Global behavior : without major problem, even withPmB(*) excepted on specific sites:• Degradations with cracks, fatigue, but also rutting sometimesobserved• Due to hazardous parameters from RAP (hardening binder,heterogeneity,…) or higher rate recycling Maintenance study + Mix design very important(questions of pertinence?) Difficulties to take into account the wear of oldaggregates on the surface friction characteristics(*) How is the real modification of the new mixing PmB binder : old and new one?
Tendencies et evolutions “Recycling easy” with the use of WMA technique (alreadyobserve in the past, high workability due to residual water bring by RA) Recycling essential to respect the topics of sustainabledevelopment Steps today:• Harmonization of practices in Europe (Direct Mat project)• Writing a guide to recommend this technique by road administrators :state of the art, practical advises, specifications, prescriptions,.. Researches:• Ageing accelerated, to predict and et anticipate the behaviors on field• Recycling with high rate, reach near 100%• Performances of binder after recycling : compatibility, homogeneity ofmix (old and new binder), characterization,…• Definition of de damage criteria on old AC, to fix the “level ofrecyclable”
Conclusions‣ High diversity of AC for pavement, to answer a specifictarget needs.‣ Complementary Researches : administration – companies‣ Mix design in lab, according to the standard performancespecifications, allows a good ad equation betwwencomposition of AC and its uses :‣Structure : mechanical, rut resistances,‣Surface : workability, resistance to water, to rut‣ Surface characteristics must be record during time (difficultto assess in lab) to validate the choice of AC pavementand the durability.
Conclusions‣ BBTM, BBUM, ECF (urban uses) on roads in good structure andgeometry, present‣ High skidding resistance, Non rutting, Economic, Sustainable.‣ Formula 0/6 gap graded :‣ excellent compromise Adherence – Noise - Esthetic‣ BBM and especially BBSG (thick) BBME (high modulus)‣ structural effect, reduction of fatigue damages.‣ BBTM 0/6 : noise diminution.‣ Different AC : operational, well under control and complementary.
Withdraw of young child 11 years oldUniversal exhibition Shanghaï 2010Thanks a lot for your attention